Materials Science and Engineering C 33 (2013) 557–563
Contents lists available at SciVerse ScienceDirect
Materials Science and Engineering C journal homepage: www.elsevier.com/locate/msec
Hot pressing effect on the shear bond strength of dental porcelain to CoCrMoSi alloy substrates with different surface treatments B. Henriques a,⁎, S. Faria b, D. Soares a, F.S. Silva a a b
Center for Mechanical and Materials Technologies, University of Minho, Campus de Azurém, 4800-058 Guimarães, Portugal Department of Mathematics and Applications, Research CMAT, University of Minho, Portugal
a r t i c l e
i n f o
Article history: Received 27 March 2012 Received in revised form 2 September 2012 Accepted 2 October 2012 Available online 7 October 2012 Keywords: Dental restoration Porcelain Co–Cr alloy Shear bond strength Hot pressing
a b s t r a c t The purpose of this study was to evaluate the effect of hot pressing on the shear bond strength of a CoCrMoSi alloy to a low-fusing feldspathic porcelain, for two types of surface treatments: polished and grit-blasted. Moreover, the shear strength of hot pressed porcelain was also compared with that of conventional vacuum sintered porcelain. Bond strength of metal–porcelain composites were assessed by the means of a shear test performed in a universal test machine until fracture. Fracture surfaces and interfaces were investigated by optical microscope, stereomicroscope and SEM/EDS. Data was analyzed with Shapiro–Wilk test to test the assumption of normality. The 2-way ANOVA followed by Tukey HSD multiple comparison test was used to compare shear bond strength results and the t-test was used to compare the porcelain shear strength (p b 0.05). Hot pressed specimens exhibited signiﬁcantly (p b 0.001) higher bond strength values than those obtained by conventional PFM technique. Signiﬁcant differences (p b 0.001) were found in the shear bond strength between grit-blasted and polished specimens. Signiﬁcant differences (p b 0.05) were also found between the shear strength of vacuum sintered and hot pressed porcelain. This study revealed that metal–ceramic bond strength is maximized for hot pressed porcelain onto rough metal substrates, with lower variability in results. Hot pressing technique was also shown to enhance the cohesion of porcelain. © 2012 Elsevier B.V. All rights reserved.
1. Introduction Metal–ceramic restorations comprise the union of a ceramic (feldspathic porcelain) to a metal substructure, through the fusion of ceramic onto the metallic substructure, hence the common name, porcelain-fused-to-metal (PFM) restorations. The success of this system relies on the strength provided by the metal substructure and by esthetics coming from ceramic, which mimics the toothlike appearance . This system is currently used in metal–ceramic dental prostheses for dental restorations (anterior and posterior crowns and ﬁxed partial dentures). All-ceramic restorations have gained prominence in recent years due to their enhanced esthetic properties . Among the materials available for ceramic-cored restorations, zirconia is pointed to as a very promising material due to its enhanced mechanical and esthetic properties [2,3]. They are though more used in single crowns and short-span partial dentures (pre molars and anterior teeth) because of their higher susceptibility to fracture on molars. The veneering porcelain chipping from zirconia-cored restorations is considered the major problem with this type of restoration [2,4]. For comparison, the incidence of ceramic veneer chipping from the zirconia core is
⁎ Corresponding author. Tel.: +351 253510220; fax: +351 253516007. E-mail address: [email protected]
(B. Henriques). 0928-4931/$ – see front matter © 2012 Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.msec.2012.10.001
8%–10% in 1–2 years while the rate of chipping with PFM is in the range of 4–10% at 10 years . Cobalt–chromium alloys are very popular alloys that are used to produce partial denture frameworks. They have the advantage over nickel containing alloys of not creating any allergic reactions . Relative to gold alloys, it is a much cheaper alloy, hence more democratic, and has enhanced mechanical properties such as higher hardness and Young's modulus . Base metal alloys have higher melting ranges (1400–1500 °C) than gold alloys (800–1050 °C), which requires more expensive melting equipments. Base metal alloys are also generally considered technique-sensitive because processing variables such as mold temperature, temperature of the molten alloy, and the sprue size and arrangement can affect the properties of the ﬁnished casting as much as composition does . Hot pressing, also called high temperature injection molding, consists of the application of external pressure to sinter and shape the ceramic at high temperature, and was ﬁrst used in the fabrication of all-ceramic restorations such as crowns, inlays, on-lays, veneers and ﬁxed partial dentures. Recently, this technique became available also for metal–ceramic restorations . Hot pressing is characterized as avoiding large pores and promoting good dispersion of the crystalline phase within the glassy matrix, hence resulting in superior mechanical properties within the ceramics [8,9] and in ﬂawless metal– ceramic interfaces. Although few, there are some studies on the bond strength of hot pressed porcelain to metal dental substructures.
B. Henriques et al. / Materials Science and Engineering C 33 (2013) 557–563
Schweitzer et al. (2005)  and Venkatachalam et al. (2009) , performed comparative studies on the bond strength of ceramic pressed to metal versus feldspathic porcelain fused to metal, although the pressable ceramic they used was indicated for all-ceramic restorations and not for metal–ceramic ones. They found no differences between the two techniques for the tested alloys, nickel–chromium vs. gold–palladium and cobalt–chromium vs. gold–palladium, respectively. Ishibe et al. (2011)  performed a study involving recently developed heat pressable ceramics for metal–ceramic restorations, and found no differences in the bond strength between the conventional layering and the heat pressing process. Henriques et al. (2011a)  found signiﬁcant differences in metal–ceramic bond strength between hot pressed and conventional porcelain fused to metal (gold based alloy). Unlike the other studies, Henriques et al. (2011a)  used porcelain in powder form and not in ingot form. The aim of this study was to assess the inﬂuence of hot pressing on the metal–ceramic bond strength, between a base metal alloy (CoCrMo) and a conventional low-fusing feldspathic porcelain, and for two types of surface treatments.
2. Material and methods For this work a CoCrMoSi dental alloy (Nobil 4000, Nobilmetal, Villafranca d'Asti, Italy) and a dental opaque ceramic (Ceramco3, Dentsply, York, USA) (batch number: 10004163) were used. The chemical composition of both materials is presented in Tables 1 and 2. Metal substrates (n = 20) were obtained by lost wax process casting in an arc melting furnace, (Degumat 2033, Degussa, Germany). Metal rods approximately 4.5 mm of diameter and 40 mm length were produced. After divesting, metal rods were cut into several metal substrates with 4 mm height using a precision cut-off machine (Minitom, Struers). Porcelain was bonded to metal substrates by two routes: conventional porcelain fused to metal (PFM) and hot pressing (HP). Two types of metal surface treatment were tested: polished surface and rough surface. First, all substrates were ground until 1200-grit sandpaper. Polished substrates were ground with 2400 grit-sandpaper and rough ones were grit-blasted with Ø110 μm alumina grains at a pressure of 3 bar (Protempomatic, Bego, Germany). All substrates were ultrasonically cleaned in an alcohol bath for 10 min and rinsed in distilled water for another 10 min to remove contaminants. They were dried with adsorbent paper towels. It was not performed any preoxidation surface treatment to the alloy before porcelain bonding. To produce PFM specimens an acrylic template was used to ensure that the porcelain height was the same for all specimens (4 mm). Porcelain was applied to metal substrates in the form of a creamy paste resulting from the addition of distilled water to porcelain powders in the ratio of 1:2 (water:porcelain). The excess of water was removed using an adsorbent paper and, after the porcelain condensing, metal– porcelain sets were carefully moved to a furnace (Vita 900, Vita, Bad Säckingen, Germany) and vacuum sintered (1 mBar) at 970 °C and at a heat rate of aprox. 70 °C/min, following the porcelain manufacturer's speciﬁcations. HP specimens were obtained by pressing the porcelain powders onto the metal substrate in a graphite die under vacuum (~10−2mBar) at a temperature of 970 °C, and at a pressure of ~20 MPa (Fig. 1). The cavity of the graphite die was veneered with zirconium dioxide to avoid carbon diffusion to specimens. The heat rate was 70 °C/min and after a Table 1 Base alloy composition (wt.%) (according to the manufacturer).
Table 2 Porcelain chemical composition (wt.%). SiO2 Al2O3 K2O 41.3 14.5
SnO2 ZrO2 CaO P2O5 Na2O Others
MgO, SO3, ZnO, Cr2O3, Fe2O3, CuO, Rb2O
2 minute stage at 970 °C, the power of the induction heating furnace was shut down. The die cooled naturally. In order to determine the effect of hot pressing on the porcelain strength, it was performed a complementary shear test to cylindershaped porcelain specimens (Ø 4.5 × 4 mm) obtained by two routes: conventional vacuum sintering (VS) and hot pressing (HP). 2.1. Shear tests The shear bond strength tests were carried out at room temperature and performed in a universal testing machine (Instron 8874, MA, USA), with a load cell of 25 kN of load capacity and under a crosshead speed of 0.5 mm/s. Tests were performed in a custommade stainless steel apparatus (Fig. 2) similar to that described by Henriques et al. (2011a) . The shear bond strength (MPa) was calculated dividing the highest recorded fracture load (N) by the cross sectional area of the bonded porcelain (mm 2). 2.2. Analysis of the metal–porcelain interface and failure mode The metal–ceramic interface as well as representative fracture surfaces were evaluated by optical microscope (Axiotech, Carl Zeiss, USA) and SEM/EDS (Nova 200, FEI, Oregon, USA). For interface analysis, the specimens were embedded in auto-polymerizing resin, ground ﬁnished to 1200 grit SiC sand-paper and polished with diamond paste ﬁrst with 6 μm and ﬁnally with 1 μm felt disk. Morphologic and chemical analyses were also performed. The elemental distribution across the metal–ceramic interface was determined by using line scan EDS analysis (20 points on the metal side and 20 points on the porcelain side). The specimens' failure modes were classiﬁed as: (1) adhesive, if no remnants of ceramic were found in the metal surface; (2) cohesive, if fractures occurred within the ceramic side; (3) mixed, if remnants of ceramic were found on the metal surface. 2.3. Statistical analysis Data were analyzed using SPSS statistic software (Release 18.0.0 for Windows). The Shapiro–Wilk test was ﬁrst applied to test the assumption of normality. Differences between processing type and surface treatment factors in the shear bond strength results were compared using 2-way ANOVA followed by Tukey HSD multiple comparison test. Differences between hot pressed (HP) and conventional vacuum sintered (VS) porcelains in terms of shear strength were tested using t-test. P values lower than 0.05 were considered statistically signiﬁcant in the analysis of the results. 2.4. Metal surface characterization The average surface roughness (Ra) of both types of specimens (polished and grit-blasted) was measured using a proﬁlometer (Mahr S5P, Germany). Two orthogonal measurements of 4 mm length on the surface of each sample were made. 3. Results
The results of the metal–ceramic shear bond strength tests performed for different processing and surface conditions are plotted
B. Henriques et al. / Materials Science and Engineering C 33 (2013) 557–563
Fig. 1. Hot pressing procedure: 1 – Die cavity is painted with zirconium oxide; 2 — Metal substrate is placed in die cavity. 3 — Porcelain powders are placed in die cavity. 4 — Hot pressing (pressure + temperature) metal–porcelain set.
in Fig. 3. The conventional PFM technique yielded lower mean bond strength values than hot pressing (HP) technique, regardless of the surface treatment used (polished (P) or grit-blasted (GB)). The results of 2-way ANOVA for the experimental conditions are presented in Table 3. The mean bond strength values were signiﬁcantly affected by the processing type (p b 0.001) and surface treatment (p b 0.001). The interaction between the processing type and surface treatment were statistically signiﬁcant (p b 0.001). The results of Tukey's multiple comparison test demonstrated that when the surface treatment was GB the HP processing type showed signiﬁcantly higher results than the PFM processing type (p b 0.05) and when the surface treatment was P the HP processing type also showed signiﬁcantly higher results than the PFM processing type (p b 0.05). When the processing type was PFM the GB surface treatment showed significantly higher results than the P surface treatment (p b 0.05). (See Table 5 and Fig. 3).
Fig. 2. Cross-section schematic of the shear test device (A: external part; B internal part). The specimens' dimensions are also shown.
In terms of processing condition, hot pressed porcelain (HP) displayed a signiﬁcantly higher strength than that of conventional vacuum sintered (VS) porcelain (t-test, p b 0.001). (See Fig. 4 and Table 4). Specimens were classiﬁed under their failure types as adhesive or mixed. All polished specimens (PFM/P and HP/P) as well as 80% of PFM/GB specimens, exhibited adhesive failure. A mixed failure type was observed for 20% of PFM/GB specimens, which showed remnants of ceramic on the metal's surface after fracture. Fig. 5 shows an EDS line scan analysis (in white) for PFM and HP specimens. This analysis shows element concentration proﬁles at the metal–porcelain interaction zone. Results show no diffusion of Co, Cr and Mo into porcelain. However, it is possible to see that Cr is present in the oxide layer formed on metal surface. Regarding porcelain elements, extensive diffusion of all its elements (O, Si, Al, K, Sn, Na, Ca, Mg) into metal was observed. Special attention must be given to oxygen, in the metal zone, which was detected in a higher concentration. The surface roughness measurements revealed that grit-blasted (GB) specimens presented approximately ten times rougher surface than polished (P) ones, with Ra=0.58 ±0.01 μm and Ra =0.05±0.01 μm, respectively.
Fig. 3. Metal–ceramic shear bond strength results for each combination of processing type (PFM — porcelain-fused-to-metal; HP — hot pressing) and surface treatment (P — polished; GB — grit-blasted).
B. Henriques et al. / Materials Science and Engineering C 33 (2013) 557–563
Table 3 Two-way ANOVA results according to metal–ceramic shear bond strength data.
Processing type Surface treatment Interaction Total
1 1 1 19
20280.43 16172.52 5141.40 45661.62
20280.43 16172.53 5141.40
79.78 63.62 20.23
1.29E-7 5.76E-7 3.66E-4
Statistically signiﬁcant at a level of p b 0.05. df: degrees of freedom; SS: sum of squares; MS: mean square; F: F-ratio; p: p-value.
Table 5 Mean ± standard deviation (SD) of the shear bond strength results (MPa). Experimental conditions Processing type
Surface treatment Polished PFM HP Mean ± SD
Grit blasted a,b,c
20.60 ± 11.63 116.36 ± 12.08b 68.48 ± 51.69e
Mean ± SD a,d
109.55 ± 26.98 141.17 ± 2.85c,d 125.36 ± 24.59e
65.07 ± 50.80f 128.76 ± 15.47f
Same superscript letters indicate signiﬁcant differences (Tukey's test, α = 0.05).
4.3. Hot pressing 4. Discussion 4.1. Materials This study evaluated the effect of hot pressing on the shear bond strength of CoCrMoSi alloy–porcelain composites and made a comparison of conventionally obtained porcelain fused to metal specimens subjected to different surface treatments, polished and grit-blasted. In this study the cobalt based alloy Nobil 4000 (Co–Cr–Mo–Si) was used. This alloy is mainly composed of cobalt and chromium, containing in its composition several other minor alloying elements (Mo, Si, Mn, Fe, W). The constituents of this alloy develop speciﬁc features, such as: chromium — provides strength and corrosion resistance via passivation ; molybdenum — provides a solid solution hardening and inﬂuences the alloy's coefﬁcient of thermal expansion (CTE) [5,13,14] ; iron and tungsten — provide a solid solution hardening to the alloy [5,13]; silicon — imparts good casting properties and increases alloy ductility . The Ceramco3 porcelain is a high-fusing, leucite based porcelain, used for metal–ceramic and all ceramic restorations. It is characterized by good mechanical properties  and is compatible with high noble, noble and predominantly base alloys.
4.2. Shear bond strength test There are several available ways to measure metal–ceramic bond strength. Among the most common mechanical tests are the shear test, the Schwickerath crack initiation test used in ISO 9693:1999, the three-point-ﬂexure test, the four-point-ﬂexure test and the biaxial ﬂexure test. The shear bond strength test results are characterized by not being inﬂuenced by the Young's Modulus of the alloy as happens for bending tests [17,18] and by its suitability for evaluation of metal–ceramic bonds . Special attention must be paid to the device conﬁguration because it can largely inﬂuence results. For instance, the shear device composed of a knife without a groove, generates great local stresses in the porcelain caused by small area of contact that can lead to the porcelain failure. Failure at the interface can be triggered by a cohesive failure in the porcelain and consequent propagation through the interface. The test device used in this study consisted of a piston-type shear device with half loop loading which reduces the stress concentration magnitude adjacent to the interface. This is considered an improved loading condition compared with concentrated force application at a single point (knife without a groove) or distributed only over a single layer . Based on these facts, many authors used this test conﬁguration in metal–ceramic bond strength characterization [21–25].
This study involves a base metal alloy and a hot pressed veneering porcelain in powder form. Few studies can be found in literature on low-fusing, leucite-based pressable ceramics to metals [7–10]. Ishibe et al. (2011)  tested the recently developed glass–ceramic pressed to metal cores, using the lost wax technique. Other authors [8,10] have tested veneering pressable ceramics, designed for all-ceramic restorations, in hot pressed metal–ceramic restorations. In this study, the hot pressed specimens showed signiﬁcantly (pb 0.05) higher shear bond strength than conventional PFM specimens. Conversely, Venkatachalam et al. (2009)  and Schweitzer et al. (2005)  found no signiﬁcant differences (p> 0.05) in metal– ceramic bond strength between ceramic pressed to metal and feldspathic porcelain fused to metal, either for noble or other base alloys. They pointed out some factors that could have inﬂuenced results, such as: the additional steps of divestment and sprue removal of pressed ceramic samples, and the excessive CTE mismatch between pressed ceramic and metal (>1 × 10−6 1/°C). The statistical analysis of bond strength data revealed signiﬁcant differences (pb 0.05) between hot pressed (HP) and porcelain fused to metal (PFM) specimens and between polished (P) and grit-blasted (GB) specimens (Table 3). The enhanced bond strength of GB specimens relative to P ones is explained by addition of surface roughness resulting from the grit-blasting treatment. Surface roughness plays a very important role in the adhesion of metal–ceramic systems and has been considered one of the most effective treatments for improving bond strength . This effect is owed to the mechanical retention that occurs as the ceramic ﬂows onto the rough metal surface, creating a Velcro-like effect (Fig. 6C and D), thus improving the adhesion between the two materials . A rough metal–ceramic interface also corresponds to a greater surface area where chemical bonds can be
Table 4 Mean ± standard deviation (SD) of the shear strength of porcelain processed by two routes, hot pressing and vacuum sintering (MPa). Processing route
Porcelain shear strength
Hot pressing (HP)
Vacuum sintering (VS)
182.06 ± 19.98
112.16 ± 21.73
Fig. 4. Porcelain shear strength results for different processing conditions (VS — conventional vacuum sintering technique; HP — hot pressing).
B. Henriques et al. / Materials Science and Engineering C 33 (2013) 557–563
Fig. 5. EDS line analysis of metal/ceramic interface showing the inter-diffusion of elements in (A) porcelain-fused-to-metal and (B) hot pressed specimens.
established. Along with the mechanical bonding, chemical bonding is also very important in the formation of strong bonding [26–28]. The chemical bonding across the interface is reported in the literature as being covalent and ionic . The chemical bonds between metal and ceramic are formed at the ceramic ﬁring process where ceramic is taken above its glass transition temperature such that it can ﬂow and fuse with the oxides at the metal surface by migration of the oxides into the ceramic. It must be pointed out that rough surfaces can also reduce adhesion in cases where the ceramic does not penetrate into the surface
and voids are formed at the interface. This may occur when metals are poorly wetted by the porcelain or when the porcelain is not properly ﬁred. These problems were shown to be overcome by the hot pressing technique, as the higher bond strength results of HP specimens demonstrate when compared to PFM ones. The imposed overpressure produced by hot pressing technique enforces a ﬂawless interface between metal and ceramic, as shown in Fig. 6B and D. The low bond strength results exhibited by PFM/P specimens are explained by a poor wetting of the polished metal surface by the porcelain. This effect is conﬁrmed by the detection of some gaps at the
Fig. 6. Metal–ceramic interface micrographs of porcelain-fused-to-metal (A — polished; C — grit-blasted) and hot pressed (B — polished; D — grit-blasted). The arrows indicate processing defects at the interface.
B. Henriques et al. / Materials Science and Engineering C 33 (2013) 557–563
metal–porcelain interface (Fig. 6A). For metal–ceramic bonding to occur it is important to wet the metal with the porcelain and in general, molten porcelain does not wet metals readily . Literature also reports that rough surfaces are often easier to wet than smooth surfaces . A good wetting, observed for low contact angles (θ b 90°) indicates the interaction between surface atoms in the metal with the ceramic . Accordingly, PFM/GB specimens presented greater bond strength values than PFM/P due to the presence of a greater surface roughness, Ra= 0.58 ± 0.01 μm vs. Ra = 0.05 ±0.01 μm. Fig. 6C shows the PFM/GB specimens interface where some porosity was detected at the metal–ceramic interface and within the porcelain resulting from processing ﬂaws (see arrows in Fig. 6C). HP/P specimens showed signiﬁcantly greater bond strength values relative to PFM/P despite both specimens exhibited polished surfaces. In this case, hot pressing technique solved the wetting problems that affected PFM/P specimens and allowed the formation of chemical bonds between metal and porcelain and, perhaps, some micromechanical bonds too (Fig. 6A, B). The HP/GB specimens displayed greater bond strength results under all tested conditions. Here, the advantages of hot pressing technique were added to the beneﬁts of a rough surface, resulting in a strong and ﬂawless interface. It should be highlighted that HP/GB specimens exhibited the least standard deviation within all tested specimens, similar to what was reported by Henriques et al. (2011a)  in a study involving a gold based alloy. The lower variability of results observed for HP/GB specimens can represent the manufacturing of more reliable restorations with greater reproducibility. In order to guarantee that thermal based pre-stress state at interface would not differ from PFM to HP specimens, equivalent heating and cooling rates were applied in both processes. The specimens' geometry was selected based on its simplicity and its broad use in similar studies for metal–ceramic bond strength assessment [11,21–25,32]. As stated before, a complementary study was conducted to assess the inﬂuence of hot pressing on the porcelain strength and a signiﬁcant (p b 0.05) increase in the porcelain shear strength was veriﬁed for hot pressed (HP) porcelain in comparison with vacuum sintered (VS) porcelain. This ﬁnding is in accordance with literature that reports some advantages of pressable ceramics over traditional porcelains, namely higher compressive strengths and higher ﬂexural strength, which are explained by an increased presence of uniformly distributed leucite phase [9,33]. Concerning the practical application of the hot pressing technique to the fabrication of metal–ceramic restorations, it has been reported in literature to be simpler and quicker than some of the conventional techniques available and to produce acceptable marginal accuracies [8,34]. Moreover, all issues related to the high rate of contraction of porcelain (~ 20%) in conventional ﬁring systems are avoided by the hot pressing technique [8,35].
4.4. Fracture type analysis Two fracture types were registered after specimen testing: mixed and adhesive failure. Except for the PFM/GB specimens, which exhibited 20% of mixed failure, all the other specimens exhibited 100% adhesive failures. Considering this fracture type pattern, no correlation can be established between the fracture type and the bond strength results. The same ﬁndings were reported by other authors for manifold processing and base material types. Henriques et al. (2011a)  found no correlation between the type of failure and the bond strength in a study involving conventional fused porcelain (PFM) and hot pressing (HP) for a gold based alloy. de Melo et al. (2005)  determined metal–porcelain bond strength for Ni–Cr and Co–Cr base alloys, and have not found a correlation between the two factors either. Akova et al. (2008)  evaluated the bond strength of laser sintered (Co–Cr) and cast base metal alloys (Ni–Cr
and Co–Cr) and were not able to establish any relation between failure type and bond strength results. The greater cohesive strength of hot pressed porcelain could have accounted for the 100% adhesive failure type veriﬁed in hot pressed specimens, despite the good metal–ceramic bond strength that was exhibited. Therefore, this can suggest that the bonding between metal and porcelain was not as effective as the enhanced cohesive strength of porcelain. 4.5. EDS analysis In order to characterize the atom diffusion phenomenon at the metal–ceramic interface, an EDS line scan analysis was performed at that site. Fig. 5 shows an oxide layer formed at the metal–ceramic interface that was formed during the porcelain ﬁring cycle since the alloy was not subjected to a preoxidation heat treatment in any of the hot pressed or porcelain fused to metal specimens. Examining the element diffusion proﬁles, one can see that the oxide layer is composed of several elements coming from metal and ceramic. Other studies indicate that this layer is commonly composed of a large quantity of Cr2O3 . Unlike Anusavice et al.'s (1977)  ﬁndings, no Co or Cr accumulation was registered at the interface. The lack of a signiﬁcant presence of Cr at the interface can be related to the absence of a preoxidation heat treatment to the alloy together with the porcelain's ﬁring cycle performed under vacuum, which could have caused some surface chromium volatilization . The presence of porcelain elements such as Si, Al, Ca, Na, Sn and Oxygen, on the metal side to a great extent, suggests a considerable width of diffusion zone. The present study demonstrates the beneﬁts that hot pressing technique can provide to the performance of a metal–ceramic restoration, especially in terms of greater metal–ceramic adhesion and porcelain fracture toughness. These ﬁndings were obtained by static mechanical tests, which do not correspond to the clinical conditions at which they are subjected in the oral cavity. Therefore, future tests should include metal–ceramic bond stress assessment after thermal and mechanical cycling in order to better simulate real operating conditions of dental materials. 5. Conclusions From this study, the following conclusions can be drawn: 1. Hot pressing (HP) technique signiﬁcantly (pb 0.05) improved metal– ceramic bond strength relative to conventional porcelain fused to metal (PFM) technique; 2. Hot pressing technique (HP) provided to the porcelain signiﬁcantly (p b 0.05) higher shear strength relative to that obtained by the conventional vacuum sintering technique; 3. Grit-blasting (GB) surface treatment signiﬁcantly (pb 0.05) improved metal–ceramic bond strength regardless of the type of processing technique that was used, hot pressing (HP) or conventional porcelain fused to metal (PFM) techniques. Acknowledgments This work has been supported by PhD grant of FCT (Portuguese Foundation for Science and Technology) with the reference SFRH/ BD/41584/2007. Special thanks to DentalCastro — Prosthetic Laboratory for their contribution in this work. References  K.J. Anusavice, in: Phillips' science of dental materials, 11th ed., W.B. Saunders, Philadelphia, 2006, pp. 621–654.  F. Zarone, S. Russo, R. Sorrentino, Dent. Mater. 27 (2011) 83–96.
B. Henriques et al. / Materials Science and Engineering C 33 (2013) 557–563  A. Vichi, C. Louca, G. Corciolani, M. Ferrari, Dent. Mater. 27 (2011) 97–108.  T.E. Donovan, E.J. Swift Jr., J. Comp. 1 (2009) 4–6.  H.W. Roberts, D.W. Berzins, B.K. Moore, D.G. Charlton, Int. J. Prosthodont. 18 (2009) 188–194.  R.G. Craig, J.M. Powers, in: Restorative dental materials, 11th ed., Mosby, 2002, pp. 480–492.  M. Ishibe, A.J. Raigrodski, B.D. Flin, K.H. Chung, C. Spiekerman, R.R. Winter, J. Prosthet. Dent. 105 (2010) 29–37.  B. Venkatachalam, R. Goldstein, M.S. Pines, E.L. Hittelman, Int. J. Prosthodont. 22 (2009) 94–100.  J.L. Drummond, T.J. King, M.S. Bapna, R.D. Koperski, Dent. Mater. 16 (2000) 226–233.  D.M. Schweitzer, G.R. Goldstein, J.L. Ricci, N.R. Silva, E.L. Hittelman, J. Prosthodont. 14 (2005) 239–247.  B. Henriques, D. Soares, F. Silva, J. Mech. Behav. Biomed. Mater. 4 (8) (2011) 1718–1726.  M. Metikoš-Huković, R. Babić, Cor. Sci. 49 (2007) 3570–3579.  W.L. Mankins, S. Lamb, in: Metals Handbook, Properties and selection: Non ferrous alloys and special-purpose materials, vol. 2, ASM International, Metals Park, OH, 1990, pp. 428–445, (ed10).  P. Crook, in: Metals Handbook, Properties and Selection: Non ferrous alloys and special-purpose alloys, vol. 2, ASM International, Metals Park, OH, 1990, pp. 446–454, (ed10).  J.F. McCabe, A.W.G. Walls, in: Applied dental materials, 9th ed., Blackwell Publishing, 2008, p. 71.  A.S. Rizkalla, D.W. Jones, Dent. Mater. 20 (2004) 198–206.  I.A. Hammad, Y.F. Talic, J. Prosthet. Dent. 75 (1996) 602–608.  I.A. Hammad, R.S. Stein, J. Prosthet. Dent. 65 (2) (1991) 169–179.  K.J. Anusavice, P.H. Dehoff, C.W. Fairhurs, J. Dent. Res. 59 (1980) 608–613.
 P.H. DeHoff, K.J. Anusavice, Z. Wang, Dent. Mater. 11 (1995) 126–131.  T. Akova, Y. Ucar, A. Tukay, M.C. Balkaya, W.A. Brantley, Dent. Mater. 24 (2008) 1400–1404.  J.G. dos Santos, R.G. Fonseca, L.G. Adabo, C.A.S. Cruz, J. Prosthet. Dent. (2006) 165–173.  V.Z.C. Vásquez, M. Öscan, E.T. Kimpara, Dent. Mater. 25 (2009) 221–231.  R.M. de Melo, A.C. Travassos, M.P. Neisser, J. Prosthet. Dent. 93 (2005) 64–69.  S.M.M. Salazar, S.M.B. Pereira, V.Z.V. Ccahuana, S.P. Passos, A.D. Vanderlei, C.A. Pavanelli, M.A. Bottino, Acta Odontol. Latinoam. 20 (2) (2007) 97–102.  W.C. Wagner, K. Asgar, W.C. Bigelow, R.A. Flinn, J. Biomed. Mater. Res. 27 (1993) 531–537.  J.R. Mackert, R.D. Rindle, E.E. Parry, A.L. Evans, C.W. Fairhurst, J. Dent. Res. 67 (1988) 474–478.  J.R. Mackert, E.E. Parry, D.T. Hashinger, C.W. Fairhurst, J. Dent. Res. 63 (1984) 1335–1340.  E.C. Marboe, W.A. Weyl, J. Appl. Phys. 20 (1949) 124.  J.S. Shell, J.P. Nielsen, J. Dent. Res. 41 (1962) 1424–1437.  C.S. Smith, Metals Technol. 15 (1948).  B. Henriques, D. Soares, F. Silva, Mater. Sci. Eng. A 528 (2011) 1415–1420.  J.R. Kelly, Annu. Rev. Mater. Sci. 27 (1997) 443–468.  E.B. Goldin, N.W. Boyd III, G.R. Goldstein, E.L. Hittleman, V.P. Thompson, J. Prosthet. Dent. 93 (2005) 143–147.  D.G. Grossman, Dent. Clin. North Am. 29 (1985) 725–739.  J.R. Mackert, R.D. Rindle, C.W. Fairhurst, J. Am. Dent. Assoc. 60 (1981) 377–381.  K.J. Anusavice, J.A. Horner, C.W. Fairhurst, J. Dent. Res. 56 (1977) 1045.  E. Krasicka-Cydzik, Z. Okisiuta, J.R. Dabrowski, J. Mater. Sci. Mater. Med. 16 (2005) 197–202.